Helsinki University of Technology
Department of Mechanical Engineering Puumiehenkuja 3 A
P.O.Box 4200 FIN-02015 HUT Finland
Dissertation for the degree of Doctor of Science in Technology to be presented with due permission for public examination and debate in Council room at Helsinki University of Technology (Espoo, Finland) on the 23rd
of November, 2001, at 12 o'clock noon.
Virkkunen, Iikka. Thermal fatigue of austenitic and duplex stainless steels. Acta Polytechnica Scandinavica, Mechanical Engineering Series No. 154, Espoo 2001, 115 pp. Published by the Finnish Academies of Technology
Keywords: thermal fatigue, austenitic stainless steel, duplex stainless steel, residual stress, Barkhausen noise, fatigue crack growth
Thermal fatigue behavior of AISI 304L, AISI 316, AISI 321, and AISI 347 austenitic stainless steels as well as 3RE60 and ACX-100 duplex stainless steels was studied. Test samples were subjected to cyclic thermal transients in the temperature range 20 – 600°C. The resulting thermal strains were analyzed with measurements and numerical calculations. The evolution of thermal fatigue damage was monitored with periodic residual stress measurements and replica-assisted microscopy. The elastic strains of the ferrite phase in duplex stainless steels were studied using Barkhausen noise. Finally, destructive analyses including fractographic scanning electron microscopy (SEM) studies and transmission electron microscopy (TEM) analyses were performed.
The surface residual stresses changed markedly during the first load cycles. In the austenitic stainless steels yielding during the rapid cooling resulted in compressive residual stresses from -200 MPa (20 – 300°C temperature cycle) to -600 MPa (20 – 600°C temperature cycle). After 10 cycles the residual stresses stabilized and then started to relax due to crack formation. Cracks were seen to initiate from persistent slip bands (PSBs) and in 3RE60 from MnS inclusions. In duplex stainless steels the phase boundaries retarded crack growth markedly.
In the austenitic stainless steels, the fracture surfaces of thermal fatigue cracks showed extensive striation formation, i.e. they were similar to mechanical fatigue. The dislocation density was lower than expected based on mechanical fatigue data. Dislocation tangles and occasional cell tendency was observed. In duplex stainless steels the plastic deformation concentrated to the austenite phase.
The obtained thermal fatigue data were compared with mechanical fatigue data from literature and with the ASME design curve. The ASME design curve was found to give safe design life, although the remaining safety factor on strain is decreased to 1.5. The total strain (elastic+plastic) caused by thermal loading was solved with linear-elastic FE-analysis. Thermal fatigue crack growth was predicted successively using total strain solution of an uncracked component and a strain-based growth model:
da dN C tota m = 7 7 ∆ε , where C7=1.6 and
m7=1.3 for the studied austenitic stainless steels.
The model is applicable to small fatigue cracks (0.05 - 4 mm) growing in varying temperature and strain fields and is temperature-independent in the studied range.
© All rights reserved. No part of the publication may be reproduced, stored in a retrieval system, or transmitted, in any form of by any means, electronic, mechanical, photocopying, recording, or otherwise, without the prior written permission of the author.
The research work presented in this thesis was mainly accomplished as a part of the research project "Thermal Fatigue Mechanisms" financed by TEKES, Fortum Nuclear Services Ltd., Fortum Oil & Gas Oy, Metso Paper Oy, Outokumpu Poricopper Oy, and Teollisuuden Voima Oy. The steering committee of the project also gave valuable comments and suggestions during my work. The support is gratefully acknowledged. The financial support of Imatran Voiman Säätiö and KAUTE (Laura & Aarne Karjalainen fund) is also acknowledged. I am deeply grateful to professor Hannu Hänninen for the advice and unlimited expertise he provided for my guidance. Numerous co-workers and friends also offered their help and support. I wish to express my gratitude to Mika Kemppainen for the fruitful collaboration, for Sergiy Smuk, Jaakko Virkkunen, and Ville Virkkunen for their encouragement and perceptive comments on my thesis, to Wade Karlsen for advice on the grammar of the thesis, to Laura Taivalaho for TEM work and help with the grammar of the thesis, to Pertti Nenonen for the exquisite TEM work, and for the workers of the Laboratory of Engineering Materials for creating a fruitful and always enjoyable working atmosphere. I also wish to extend my gratitude to the pre-examiners of this work, Prof. Gary Marquis and Dr. Arttu Laitinen for their very valuable and constructive criticism.
Finally, I wish to express my deepest gratitude to my wife Päivi and to my newborn daughter, who made my life outside my work exceedingly rewarding.
Otaniemi, June 2001
CONTENTSAbstract 2 Preface 3 Contents 4 Original features 6 Nomenclature 7
1 Introduction – current understanding of thermal fatigue 10
1.1 Thermal stresses ...11
1.2 Residual stresses ...13
1.4Dislocation structures produced by cyclic loading...15
1.5 Fatigue crack initiation ...16
1.6 Fatigue crack growth ...16
1.7 Fracture mechanics ...20
1.8 Crack growth models for fatigue design...22
1.9 Fatigue properties of austenitic and duplex stainless steels ...29
1.10Multiaxial fatigue ...32
1.11Environmental effects ...32
1.12Dynamic strain ageing ...36
1.13Thermal fatigue ...36
2 Aims of the current work 43 3 Experimental procedure 44 3.1 Materials...44
3.2 Thermal fatigue tests...46
3.3 Thermal load determination ...49
3.4Residual stress profile measurements by contour method ...49 3.5 Cyclic stress-strain tests...50
3.6 Numerical simulations...52
4Results 54 4.1 Cyclic stress-strain curves...54
4.2 Barkhausen noise measurements...55
4.3 Cyclic strain caused by thermal loading...57
4.4 X-ray measurements ...61
4.5 Contour method ...69
4.6 Build-up of surface damage...69
4.8 Dislocation structures ...77
5 Discussion 81 5.1 Cyclic thermal loads and residual stresses...81
5.2 Micromechanism of crack growth ...82
5.4Comparison of thermal and mechanical fatigue ...88
6 Conclusions 91
7 References 92
Appendix 1. Two-bar model for thermal stresses 109
Appendix 2. Derivation of equation 41 111
Appendix 3. Used FE-models 112
The experimental data and analyses of this thesis are directed towards modeling and predicting thermal fatigue damage and especially thermal fatigue crack growth in stainless steels. The following features are believed to be original:
1. Detailed study of the strains, residual stresses, dislocation structures and fatigue crack growth caused by cyclic thermal loading was performed. 2. An original method was developed to measure the elastic strains of the
ferrite phase in a two-phase ferritic-austenitic duplex stainless steel using Barkhausen noise.
3. Linear-elastic FEM solution was found to give good approximation of the total (elastic + plastic) strains in strain-controlled, thermal load case. 4. The acquired thermal fatigue data was analyzed according to the ASME
(1995) pressure vessel code. The code was found to give safe design life; the remaining safety factor on strain is 1.5.
5. It was shown that thermal fatigue crack growth in the crack depth range of 0.1 – 5 mm can be predicted using a total strain based crack growth model: da dN C tota m = 7 7 ∆ε , whereC7=1.6 and
m7=1.3 for the studied austenitic stainless steels.
6. It was shown that the model used is independent of test temperature in the studied range.
7 . Verified range of the applicability for the crack growth model was extended from mechanical fatigue to thermal fatigue and for cracks growing in varying strain and temperature fields.
A Area (m2)
a Crack depth
a0 Initial crack depth
aeff Effective crack length for the El Haddad model
b Burgers vector
C1 Parameter for the Paris law
C2 Parameter for the Paris equation used with Kε
C3 Parameter for the Tomkins model
C4 Parameter for the Solomon model
C5 Parameter for the Ahmad-Yates model
C6 Parameter for the Ahmad-Yates model
C7 Parameter for the Taira model
C8 Parameter for the Nisitani model
D Deformation zone size (µm) Plastic zone size (µm)
d Grain size of the material (µm) E Young's modulus (GPa)
Fen Fatigue life correction factor for environmentally assisted fatigue
G Energy release rate
Iβ Material constant for the Skelton model J J integral
Je Elastic part of J
Jp Plastic part of J
K Stress intensity factor (MPa m0.5)
KI Stress intensity factor for mode I loading (MPa m0.5)
KISCC Threshold stress intensity factor for stress corrosion cracking (MPa m0.5)
Kε Strain intensity factor (m0.5)
M Material constant for the Paris law m1 Parameter for the Paris law
m2 Parameter for the Paris equation used with Kε
m4 Parameter for the Solomon model
m5 Parameter for the Ahmad-Yates model
m6 Parameter for the Ahmad-Yates model
m7 Parameter for equation 40
m8 Parameter for the Taira model
N Cycle number
O' Parameter describing the effect of dissolved oxygen on corrosion fatigue q Parameter for the Haigh-Skelton model
R Load ratio (εmin/εmax)
r Radius (mm)
rI Inner radius (mm)
S Striation spacing (µm) s1 Strain hardening exponent
s2 Work hardening exponent
T Temperature (°C)
T' Temperature dependent parameter for estimating Fen
Te Equivalent temperature (°C)
Tmax Maximum temperature during a cycle (°C)
Tmin Minimum temperature during a cycle (°C)
Tt Traction vector for the J integral
t Parameter for the Gabetta model u Displacement (mm)
Vα Volume fraction of α-phase (%) Vγ Volume fraction of γ-phase (%) W Strain energy density
wc Hysteresis energy per cycle
We Elastic strain energy density
Wf Energy required for failure
Wp Plastic strain energy density
Y Geometry factor for K and Kε
∆Kth Threshold stress intensity factor range below which crack growth stops
∆σl Fatigue limit
Γ Arbitrary path surrounding the crack tip α Linear coefficient of thermal expansion (K-1)
Ferrite phase in duplex stainless steels β Material constant for the Skelton model
ε Strain (mm/mm)
ε Strain rate (s-1) ˙
ε' Parameter describing the effect of strain rate on corrosion fatigue εa Axial strain (mm/mm)
εe Elastic strain (mm/mm)
εeb Elastic biaxial strain (mm/mm)
εeq Equivalent strain for the Haigh-Skelton model (mm/mm)
εeu Elastic uniaxial strain (mm/mm)
εm Measured apparent strain (mm/mm)
εmax Maximum strain, e.g., during a cycle (mm/mm)
εmin Minimum strain, e.g., during a cycle (mm/mm)
εp Plastic strain (mm/mm)
εpb Plastic biaxial strain (mm/mm)
εpu Plastic uniaxial strain (mm/mm)
εr Radial strain (mm/mm)
εt Tangential strain (mm/mm)
εtot Total (elastic+plastic) strain (mm/mm)
εΤ Thermal expansion (mm/mm)
εσ Constrained thermal expansion (mm/mm) γ Austenite phase in duplex stainless steels ν Poisson's ratio
σ Stress (MPa)
σµ Microscopic (average) stress (MPa)
σa Axial stress (MPa)
σf Flow stress (MPa)
σM Macroscopic stress (MPa)
σmax Maximum stress during a cycle (MPa)
σphase Total average phase stress (MPa)
σt Tangential stress (MPa)
σy Yield stress (MPa)
σyc Cyclic yield stress (MPa)
σµα Microscopic (average) stress in phase α (MPa)
σµγ Microscopic (average) stress in phase γ (MPa) σr Radial stress (MPa)
INTRODUCTION – CURRENT UNDERSTANDING OF THERMAL FATIGUE
Components subjected to alternating heating and cooling have been found to crack and eventually fail. This phenomenon is termed thermal fatigue. The reason for cracking is believed to be twofold. Firstly, temperature change in the material induces thermal expansion (or contraction). If surrounding material or external constraints hinder this expansion, thermal stresses arise. These cyclic thermal stresses cause fatigue similar to that of mechanical stresses. Typical components where this kind of problems arise are, e.g., power and process industry pipings where turbulent mixing of fluids causes quick thermal transients, or rotating components in the paper industry where frictional heating causes rapid temperature cycles (e.g., Dean, 2000; Hänninen & Hakala, 1981).
Secondly, at high temperatures, materials are found to exhibit time dependent deformation, i.e. creep. Failure is generated by a process combining creep and fatigue (e.g., Taira & Fujino, 1979; Zamrik, 1990; Goswami, 1999; Gandossi, 2000). Creep becomes more significant with increasing temperature and prolonged exposure. Typical components, where creep-fatigue interaction is significant include gas turbine blades and soldered joints of electric circuitry.
The motivation for this study of thermal fatigue is to enhance the reliability of affected components. The economical effects of unexpected failures can be very high, e.g., in power, process and paper industries. Failures may threaten property and even life. The existing design methods do not give adequate tools for design against thermal fatigue. In the case of thermal fatigue, the increase of safety by using heavier constructions is not only uneconomical but also often impossible. In some cases a heavy design increases the constraint to thermal expansion and thus has a negative effect on component safety.
This study is focused on the thermal fatigue in power, process and paper industries, where time-dependent effects can be presumed to be negligible (Zauter et al., 1994). The theoretical background on which the current understanding of the phenomenon is based is that of mechanical fatigue (or just fatigue) and thermal stresses.
Change in temperature induces thermal expansion in a material:
εT = ∆α T, (1)
whereεT is the thermal expansion (mm/mm),
α is the linear coefficient of thermal expansion (K-1) and
∆T is the temperature change causing the expansion (K).
If this expansion is hindered, thermal stresses arise. The magnitude of the arising stresses is such that if applied as an external load they would result in strain equal to the hindered expansion. Thermal stresses can arise because of either external or internal constraints. Internal constraints can be caused by nonuniform temperature distribution or nonuniform material properties. If the thermal stresses arise due to internal constraints, the loading is called pure thermal loading, or just thermal loading. If the stresses are due to external constraints, term thermomechanical loading is used.
The elementary theory of thermal stresses is quite well established, and several textbooks have been written on the subject (e.g., Boley & Weiner, 1960). Analytical solutions to elastic and elastic-perfectly plastic thermal stress problems in various geometries have been presented in literature (e.g., Fritz & Schenectady, 1954). For example, the thermal stresses in an elastic cylinder or tube with radial temperature distribution are given by (Boley & Weiner, 1960):
σ α ν r I O I r r r r r E r r r r r I Trdr ITrdr O
( )= −
∫1 2 2 2 2 2 (2) σ α ν t I O I r r r r r E r r r r r ITrdr ITrdr Tr o
( )= −
)+− + −
∫1 2 2 2 2 2 2 , (3)
whereσr is the radial stress (MPa),
σt is the tangential stress (MPa),
α is the linear coefficient of thermal expansion (K-1),
E is Young's modulus (GPa), ν is Poisson's ratio,
T(r) is temperature (K), r is the radius (mm),
rI is the inner radius of the tube (mm) and
rO is the outer radius of the tube (mm).
If the axial deformation of the cylinder is unconstrained, the axial stress is given by:
σ α ν σ σ a O I r r r t r E r r I Trdr T O
( )= −
)− − = +
∫1 2 2 2 , (4)
where σa is the axial stress (MPa) and the other symbols are as in equations 2
In addition to full solutions, simplified parameters for the severity of thermal transients have been proposed. Yoshimoto et al. (1999) showed that the maximum thermal stress, which develops during a quench test, can be estimated as follows:
σmax =0 705.
)−43 80. , (5)
where σmax is the maximum thermal stress during a quench test,
E is Young's modulus (GPa),
∆T is the temperature difference (K) and
α is the linear coefficient of thermal expansion (K-1).
In a two-phase material, such as duplex stainless steel, where the two phases have different thermal expansion behavior, change in temperature gives rise to strain mismatch and thermal stresses between the two phases. The resulting microscopic thermal stresses, i.e. microstresses, can be very complex. The microstresses have to be superimposed on the macroscopic stresses to give the total phase-specific stresses.
Stevens (1999) studied the effect of thermal treatment simulating welding on the corrosion fatigue life of duplex stainless steels, and found that the applied temperature cycle reduced the corrosion fatigue life of the samples. He attributed this effect to both secondary phase precipitation and residual stresses. Behnken & Hauk (1992a; 1992b) studied the effect of microstresses on fatigue behavior, and concluded rather surprisingly that, since the residual microstresses are typically much smaller than the macroscopic residual stresses, their effect can be neglected. Other sources (Pohl & Bracke, 1997; 1999) however, concluded that thermal cycling up to 900°C causes microscopic thermal strains that result in stresses exceeding the yield strength in every cycle. Because in duplex stainless steels both constituent phases are capable of plastic deformation, pure thermal cycling can accumulate macroscopic strain to the specimens (Pohl & Bracke, 1999; Fischer et al., 1990; Siegmund et al., 1993; 1995). As temperature rises, stresses in the austenite phase are shifted towards compression, and stresses in the ferrite phase towards tension, due to the greater thermal expansion of the austenite phase. During cooling the stresses are reversed. This has been found by both X-ray residual stress measurements (Kamachi et al., 1982) and numerical simulations (Siegmund et al., 1993). The microscopic thermal stresses are highly dependent on the local microstructure, i.e. local phase morphology. In order to model the phenomenon, a set of quantitative parameters are needed to describe the investigated microstructure (Siegmund et al., 1995; Silberschmidt & Werner, 1999).
In addition to external loads, thermal or mechanical residual stresses often exist in a component. These stresses result from uneven yielding during, e.g. manufacturing or thermal treatments. Residual stresses are difficult to model or measure, and they often form an unknown factor in fatigue. The residual stresses tend to fade during fatigue loading (Almer et al., 2000). Stabilized residual stresses correlate with fatigue crack initiation and fatigue life.
In a two-phase material, such as duplex stainless steels, microscopic residual stresses in the constituent phases can develop. These microstresses can result from uneven yielding of the phases during plastic deformation (e.g., Inal et al., 1999) or from uneven thermal expansion of the two phases. Irrespective of their origin, the residual stresses have strong impact on load sharing between the phases and on mechanical behavior, especially on the fatigue properties of the material. The residual stresses in a two-phase material affect the apparent thermal expansion behavior (Wang et al., 1999). The uneven yielding also causes a surface relief to develop (Polák et al., 1999).
The uneven yielding during plastic deformation gives rise to residual microstresses. The total stress in a phase is then the sum of the micro- and macrostresses:
σphase =σM +σµ, (6)
whereσphase is the total (average) stress in a phase,
σM is the macroscopic stress and
σµ is the microscopic (average) stress in a phase.
In a randomly oriented microstructure the microscopic stresses of the constituent phases are related through the equilibrium condition:
Vα µασ +Vγ µγσ =0, (7)
whereVα and Vγ are the volume fractions of phases α and γ and σµα and σµγ are the (average) microstresses in phases α and γ, respectively.
Johanson & Odén (1999; 2000a; 2000b) studied the load sharing between the austenite and ferrite phase in nitrogen containing duplex stainless steels. They concluded that the hardness and the yield strength of the austenite phase are higher than those of the ferrite phase. Despite its greater strength, more plastic deformation occurs in austenite than in ferrite because of the compressive residual stress present in the ferrite phase after cooling (Johanson & Oden, 1999; 2000a; 2000b). A higher load, therefore, is transferred through the ferritic matrix. The ratio of plastic strain in austenite to that in the ferrite increases with decreasing
nitrogen content and increasing total strain amplitude (Degallaix et al., 1995).
Plastic deformation changes the residual microstresses due to uneven yielding in the constituent phases. Moverare (2001) studied the evolution of residual stresses in uniaxial tension. The experiment was repeated in several loading directions on duplex stainless steels. He concluded that the load partitioning between the two phases is dependent on the loading direction: for loading in the rolling direction, both phases deform plastically to the same degree, while more plastic deformation occurs in the austenitic phase during loading in the transverse direction. The difference in load partitioning was attributed to crystallographic texture in the ferritic phase.
Fatigue is defined as the degradation or failure of a material caused by cyclic loads. The study of fatigue started with the so-called phenomenological models, which ignore the mechanisms by which the fatigue failure takes place, but aim to establish a tool with which the fatigue endurance of a component can be predicted. The Wöhler and Coffin & Manson plots have been the basis for fatigue design for many decades and are still used in many design codes such as the ASME pressure vessel code (1995). During the years, several improvements have been proposed to the plots (e.g., Muralidharan & Manson, 1988; Hatanaka, 1990).
At first the material properties were assumed to remain constant during the fatigue life. Especially in low cycle fatigue, this is often not the case. Cyclic loading hardens or softens the material. The change in material properties starts from the first cycles and continues to final fracture. Consequently, the monotonic material properties do not describe the material adequately, and fatigue life predictions can be improved by considering the cyclic properties (Mughrabi, 1993, 1996; Mughrabi et al., 1997). Several corrections for the Coffin-Manson model have been proposed which take into account the cyclic properties (e.g., Kliman, 1983; Mughrabi, 1996; Shi & Pluvinage, 1994; Hatanaka, 1990). Mughrabi (1996) studied the cyclic stress-strain behavior of f.c.c and b.c.c materials. He compared the cyclic properties of these materials with several life prediction models and concluded that the microstructural interpretations of fatigue behavior are still far from being comprehensive and consistent. The cyclic stress-strain curve is affected by metallurgical factors, such as mobility of screw dislocations, strain-induced martensite and dynamic strain ageing (Hatanaka, 1990). For austenitic stainless steels several constitutive models for predicting cyclic properties have been proposed (Ohno & Kachi, 1986; McDowell, 1987).
The main drawback of the phenomenological approach is that because it lacks a direct relation to the cumulating fatigue damage, it provides inadequate tools to assess the remaining safe life of a cracked component. Also, the effect of various defects from manufacturing etc. is difficult to take into account. In addition, the cyclic stresses or strains in the component may not be uniform throughout the component, which leads to retardation or acceleration of crack growth. This cannot be adequately modeled with the phenomenological approach. Despite their inadequacies, the phenomenological models still remain in many cases the only practical design method for components with small or no initial defects. Chopra & Shack (1999) note that, although the S-N curves are conventionally used to give the number of cycles to produce gross failure for given stress or strain amplitude, they would be better interpreted as specifying the number of cycles required for the formation of an "engineering" crack for example 3 mm deep.
Dislocation structures produced by cyclic loading
Numerous studies on the dislocation structures generated by mechanical fatigue in austenitic and duplex stainless steels can be found in literature. Gerland et al. (1989; 1997) fatigued AISI 316L isothermally at different temperatures ranging from 20 to 600°C. In the beginning of fatigue at a small plastic strain amplitude (εp=2x10-3), dislocation tangles and irregular
cells were found. After failure, or with greater strain amplitudes, high dislocation densities and tightly arranged dislocation structures, such as walls-and-channels, cells or corduroy, were observed. Kruml et al. (1997) found ladder-like dislocation structures in AISI 316L fatigue-tested at room temperature. This structure was explained to be responsible for the strain localization. Li & Laird (1994) also found cells and walls-and-channels dislocation structures after room temperature fatigue in an AISI 316L single crystal. Orbtlík et al. (1994) (also for AISI 316L) explained that the different dislocation structures found in austenitic stainless steels are due to their intermediate stacking fault energy (SFE). Hence the dislocation structure depends on the applied strain range. For small strain amplitudes (<10-4), the planar dislocation structures typical for low SFE
materials prevail, i.e. corduroy, dislocation alignments and planar slip bands. For high strain amplitudes (>10-3) walls-and-channels and cells
typical for high SFE materials prevail. Xia et al. (1992) studied a manganese-alloyed austenitic stainless steels and found similar dislocation arrangements. Similar dislocation arrangements are also observed in the austenite phase of duplex stainless steels. In the ferrite phase of duplex stainless steels, veins-and-channels and ladder structures are observed (Degallaix et al., 1995). In the ferrite phase, the observed dislocation structures do not change markedly with the strain amplitude.
Fatigue crack initiation
Traditionally the failure is divided into three phases: crack initiation, crack growth or propagation, and final fracture. During the initiation period, a visible crack or cracks form. The initiated cracks then grow and at some point the growing cracks have weakened the structure so much that the load bearing capacity is exceeded and final fracture occurs.
At very low load amplitudes, near the fatigue threshold, most of the life is spent on the crack initiation phase. As the load amplitudes increase, the proportion of the life spent in the propagation phase increases rapidly. The distinction between the initiation and the propagation phases is somewhat ambiguous. With the development of better methods of detecting cracks, smaller cracks have become detectable and the initiation period has shortened. Also considerable scatter now exists in the definition of initiation: it can mean cracks visible to the naked eye (in the range of 1 – 2 mm) or it can mean smallest cracks visible in the electron microscope (in the range of a few µm). It has been suggested that initiation is absent altogether and that first undetectable cracks initiate during the first load cycle (Miller, 1999). Crack initiation typically takes place at material inhomogenities. These can be for example persistent slip bands caused by cyclic loading, grain boundaries or nonmetallic inclusions. The fatigue strength depends on the "weakest link", e.g., from the largest inclusion present (Murakami & Endo, 1993; Murakami et al., 1994).
Fatigue crack growth
After crack initiation, the fatigue damage is concentrated to the highly strained area of the crack tip. In small crack lengths the crack growth rate is highly dependent on the local microstructure and coalescence of cracks (Miller 1999). After the crack length is more than about 3 times the grain size, the crack growth can be described by a single mechanical parameter (Kawagoishi et al. 2000).
Ductile metals deform plastically at the highly stressed area around the crack tip. In the area where stresses exceed the yield strength of the material, the monotonic plastic zone is formed. The plastic zone alters the stress and strain distribution at the crack tip. In the cyclic case, unloading reverses the stress direction. The changes in the stresses and strains are given by a solution identical to that of monotonic loading but with yield strain and stress replaced by twice their values (Rice, 1967). Consequently, a much smaller cyclic plastic zone forms inside the monotonic plastic zone (Figure 1). The formation of these plastic zones was also experimentally verified (e.g., Davidson & Lankford, 1976; Williams et al., 1980). Lankford et al. (1984) studied the crack tip deformation of small fatigue cracks and found that the measured crack tip opening (CTOD) and crack tip plastic zones were much larger than those predicted based on long
crack models. They concluded that the large plastic zone compared to the crack depth at least partly explained the anomalous crack growth rate of small cracks.
Figure 1. Schematic illustration of monotonic and cyclic plastic zones and stress distributions (after Rice, 1967).
The crack propagation phase is subdivided based on the plane of the crack advance. The crack can grow by two processes and corresponding planes: shear decohesion on one plane directly ahead of the crack tip, or shear decohesion of two mutually perpendicular planes inclined at about 45° to the crack plane (Miller, 1999). The former is termed stage I and the latter stage II crack growth. Stage I crack growth is mainly observed at small applied load ranges, whereas stage II is typical for high loads. Cheng & Laird (1983) suggested that the transition occurs due to work hardening on the primary slip system. The work hardening causes strain to be transferred partly to the secondary slip system. This causes persistent slip band (PSB) formation on the secondary slip system and transition from stage I to stage II crack growth. The orientation of the crystal relative to loading affects the stresses on the secondary slip system and consequently the transition behavior. The higher the stresses on the secondary slip system are, the earlier the transition to stage II crack growth occurs.
Lukásˇ & Kunz (1984) and Lukásˇ et al. (1985) studied the dislocation structures ahead of a fatigue crack tip in copper (Figure 2). They found that the high strains directly ahead of the crack tip are extended by the formation of slip bands. The crack was found to follow the path of the highest local deformation. At low amplitude loading, the zone of the cell structure ahead of the crack tip is small and the crack follows PSBs. With higher load amplitudes, the crack tip is surrounded by an extensive zone of dislocation cells which does not contain preferred paths, and the crack propagates non-crystallographically. It was also found that the crack growth rate was proportional to the local crack tip plastic strain (Lukásˇ et al., 1985).
Figure 2. Dislocation structures ahead of fatigue crack tip in copper (after Lukásˇ Aet al., 1985).
The portions of fatigue life spent in initiation, stage I and stage II of crack growth depend on the environment, material and loading (Socie & Bannantine, 1988). The fracture surface left by a stage I crack appears faceted. The facets form as the crack changes the plane of advance. By contrast, stage II cracks leave ripple-like markings, striations, which describe the crack advance by cycle. Several models have been proposed to explain the formation of striations. The blunting model, proposed by Laird & Smith (1962), is presented in Figure 3. Tomkins (1968) presented an alternative model (Figure 4). His model was criticized by Laird & de la Veaux (1977). The model was further developed in later publications (Tomkins, 1980; 1981; 1983a). The main difference between these two models is that slip is condensed to either one or several sets of PSBs ahead the crack tip. Neumann (1969), Pelloux (1969) and Vehoff & Neumann (1978) developed an alternative model for striation formation (Figure 5). In this model, the crack forms a V-shaped tip and advances by alternating slip on two slip bands. This model was supported by recent fracture surface studies and was developed further by Bichler & Pippan (1999). It should be noted, however that great variation in the appearance of fatigue striations is perceived in different materials, environments and loading conditions. Hence, it may be that a single model for their formation is not conceivable.
Figure 3. The blunting model of striation formation (after Laird & Smith, 1962).
Figure 5. The Neumann-Pelloux-Bichler model of striation formation (after Bichler & Pippan, 1999).
Striation spacing is generally considered to be an indicator of the crack advance per cycle. However, in-situ observations have revealed that, in the near-threshold regime where crack growth rate is low, this is not necessarily true. As the crack growth rate diminishes, more than one cycle is needed to form each striation. Finally, very close to the threshold the striation spacing reaches a minimum of 0.1 – 0.4 µm and is independent of the crack growth rate (Davidson & Lankford, 1992). Recently, Uchida et al. (1999) showed that the stress ratio (R) could also be determined from the fracture surface by studying the height of the striations.
At greater crack growth rates the striations give a direct indication of the crack growth rate. Since fatigue crack growth does not occur continuously, but the advancing crack (at least locally) slows or stops at microstructural barriers (Tanaka, 1989), the growth rate calculated from striation spacing is a conservative estimate. Tanaka et al. (1981) proposed a correlation between the striation spacing and ∆K-level (see sections 1.7 and 1.8): S b K E b J Eb = ∆ = ∆ 10 10 10 3 2 , (8)
whereS is the striation spacing,
b is the atomic distance or Burgers vector,
∆K is the stress intensity factor range (see section 1.7) and ∆J is the J integral range (see section 1.7).
In 1920 Griffith (1920) published his classic paper on the phenomena of rupture and flow of solids. His paper concludes that the strength of brittle glass samples was determined by the size of flaws present. He proposed that the amount of surface energy required by the growing crack
determined the stress needed to break the sample. He then concluded that the strength of a cracked plate was inversely proportional to the square root of the length of the crack present. Later Irwin (1947) generalized this idea to include energy dissipated by plastic flow and named the defined parameter energy release rate, G (Irwin, 1957). With the help of a stress solution of a cracked plate given by Westergaard (1939), it was then shown that the crack tip stresses are proportional to a quantity called the stress intensity factor, given for plane stress by:
K = EG
where K is the stress intensity factor (MPa m0.5) and G is the energy release rate (J mm-2).
In a force-controlled load case the solution of G usually gives the a
dependence noticed by Griffith (1920). In a displacement-controlled load case, the dependence of K on the crack length a can be quite different or even nonexistent, as for example in the case of displacement-controlled loading of a very long crack in an infinite plate.
The linear elastic fracture mechanics (LEFM) parameter K has been a very successful tool in describing many failure mechanisms that feature crack growth. However, with high stresses or small crack lengths the small scale yielding condition of K is violated, and K loses its validity. Rice & Rosengren (1968), Rice (1968) and Hutchinson (1968) proposed that the crack tip could be characterized by a line integral (J-integral or J) around the crack tip even in the case of plasticity exceeding the small scale yielding condition of K: J Wdy T du dxds t = − ⋅
∫Γ , (10)
where W is the strain energy density, Tt is the traction vector and
Γ is a path surrounding the crack tip.
The elastic-plastic fracture mechanics (EPFM) parameter J is directly related to K in the case of small scale yielding (Rice & Rosengren, 1968):
J K E I =
)2 2 ν . (11)
J is extensively used for crack tip characterization in inelastic load cases. In the case of thermal gradients, the conventional definition of J loses its path independence. Wilson & Yu (1979) showed that J can be calculated also in thermal stress crack problems, but the solution involves a computationally difficult area integral:
J E T x ii x T ii dA A = −
∫α ν ∂ ∂ ε ∂ ∂ ε 1 2 1 2 1 1 0 , (12) where T is temperature.
Following the analysis of Wilson and Yu (1979) the J equation for an arbitrary eigenstrain distribution can be solved and used to solve J in a residual stress field, which again involves an area integral.
Crack growth models for fatigue design
Paris et al. (1961) and Paris & Erdogan (1963) showed that the fatigue crack growth rate could be characterized with the LEFM-based parameter, ∆K: da dN K M = ∆
( )4 , (13)
whereM is a material constant and ∆K is the stress intensity range.
The empirical Paris-Erdogan equation is now by far the most used crack growth model (see Tomkins (1984) for a review of classical crack growth based fatigue analysis). Usually the exponent is also considered as a material constant or a fitting parameter and the equation is presented in the following, more general form:
dN C K
where C1 and m1 are material constants.
With very high loading the small scale yielding condition of LEFM is no longer valid and ductile tearing fracture and other fracture mechanisms take part in the process. Hence the applicability of Paris-Erdogan law is limited at high ∆K-values. With low ∆K-values the crack growth rate is observed to deviate from the Paris law (equation 14) and to decrease rapidly. This point is termed the threshold stress intensity range, ∆Kth.
Consequently, the fatigue crack growth is divided into three regimes. A schematic crack growth plot is shown in Figure 6.
Figure 6. Schematic crack growth plot with Paris parameters (after Tanaka, 1989).
At small crack lengths, the applied stress to produce a certain K-value is very high. With high stresses the plastic zone of the crack is large compared to the length of the crack and the small scale yielding condition of K is violated. Consequently, the observed crack growth rates are higher than predicted by the Paris law. Because the fatigue life spent during the early crack growth is very long, the inability of the Paris law to correctly predict the small crack growth is a serious handicap.
The limits of the linear elastic fracture mechanics were extended by the introduction of elastic-plastic fracture mechanics (see Paragraph 1.7). Similarly the limitations of the Paris law that are caused by the limitations of linear elastic fracture mechanics could be extended by the use of EPFM parameters such as J. Dowling & Begley (1976) and Dowling (1976; 1977) were among the first to test the applicability of the elastic-plastic J parameter to fatigue crack growth characterization. They concluded that for ductile materials and long cracks J characterized the crack growth for high load state and ligament plasticity. Hoshide et al. (1985) tried to correlate small crack growth with ∆J and found that with crack lengths greater than three times the grain size of the material correlation could be found. For smaller crack lengths, the coalescence of cracks caused a higher than predicted crack growth rate.
Observed fatigue crack growth depends on numerous other factors in addition to ∆K or ∆J. For example, the load ratio R, environment, microstructure, temperature, overloads, and short cracks change the crack growth rate. Elber (1970) proposed that these effects could be explained by premature crack closure, which reduces the effective ∆K. The concept has
been used widely since then. Dowling & Begley (1976) and Dowling (1976) corrected their ∆J values for crack closure, which appeared at nonzero (compressive) load in their analysis. Chen et al. (1997) concluded that both ∆J and closure-corrected ∆Jeff were successful in predicting high
temperature crack growth in AISI 304 steel. Sadananda & Vasudevan (1995) showed that crack closure is often overestimated and is not sufficient to explain the observed anomalies in crack growth. They proposed instead that fatigue crack growth is dependent upon two parameters: Kmax and ∆K (or the equivalent Jmax and ∆J) (Vasudevan et al.,
1992; 1993; Vasudevan & Sadananda, 1993; 1995a; 1995b; Sadananda & Vasudevan, 1995; 1997a; 1997b).
The main disadvantage of the K- and J-based models is the problem with predicting small crack growth and crack growth from notches (Pippan et al., 1986). In addition, the calculations required for the assessment of loading at the crack tip are often very difficult. Many analytical solutions for K are available (e.g., Murakami, 1987). For J the solutions are not that readily available. Dowling (1977) presented the following approximate J solution for small half-circular surface cracks:
J J J W a W a E s e p e p p = + = + = + + 3 2 5 0 3 2 2 5 0 1 2 1 . . . σ . σε , (15)
where Je is the elastic part of J,
Jp is the plastic part of J,
We and Wp are the elastic and plastic strain density and
s1 is the strain hardening exponent and
a is the crack depth.
Nowadays J-based design is usually based on J calculated from finite element (FE) analysis. The calculations are rather demanding due to the elastic-plastic modeling required. If the temperature is not uniform throughout the specimen, additional difficulties arise due to the area integrals present.
Several extensions and modifications have been proposed to the above mentioned crack growth laws (e.g., review by Hussain, 1997). Many of them are developed to extend the applicability of the traditional LEFM and J approaches to small crack growth and crack growth from notches. El Haddad et al. (1980) proposed that an effective crack length aeff should be
added to the crack length a when calculating ∆K of ∆J to account for the fatigue limit. The effective crack length aeff can be obtained if the threshold
stress intensity range and fatigue limit of the material are known:
aeff Kth e = ∆ ∆ σ π 2 1 , (16)
Lantaigne & Baïlon (1981) suggested an improved model for near-threshold crack growth. In their model fatigue damage was modeled to cumulate in a certain damage zone ahead of the crack tip. Lal (1994) proposed that the applicability of the Paris approach could be extended to small and near-unstable crack growth by dividing the crack growth into three regimes. The crack growth in each regime was described by a Paris type equation (equation 14) with different material constants C2 and m2.
Crack growth from notches has also been successfully predicted by replacing the stress intensity factor K with a strain intensity factor Kε (Leis, 1985; Hatanaka et al., 1989):
ε = =ε π , (17)
where Y is a geometry factor.
When the Paris law (equation 14) is used together with the strain intensity factor, the corresponding material parameters C and m have the following relationships: m1=m2 (18) C C Em 1 2 2 = , (19)
where the subscripts 1 and 2 denote parameters to be used with stress and strain intensity factors, respectively.
Liu & Kobayashi (1980) proposed the following relation based on the unzipping model for crack growth:
da dN K E J yc yc =0 02 1
( )∆ =0 02 2 . ν . σ σ ∆ , (20)
where σyc is the cyclic yield stress.
Tomkins (1968) proposed a crack growth model based on the micromechanism of fatigue crack growth (see section 1.4). The basic assumption in the model is that the crack growth rate can be calculated from the size of the crack tip deformation zone:
∆ =a εpD, (21)
where∆a is the crack advance,
εp is the applied plastic strain and
D is the deformation zone size.
D a ≈ sec π 2 . (22)
This gives the following cyclic crack growth law (Tomkins 1968):
dN =C3∆εpa, (23)
whereC3 is a material constant.
In later publications, the equation was modified to (Tomkins 1980; 1981; 1983a): da dN C pa t f = 3 2 2 ∆ε σ σ , (24)
whereσt is the stress amplitude and
σf is the material flow stress.
Solomon (1972) proposed the following, more generalized crack growth law for high strain fatigue:
da dN C p a m = 4 4 ∆ε , (25)
whereC4 and m4 are material constants and
∆εp is the bulk plastic strain range.
Equation 25 cannot be used for high cycle fatigue, where εp<<εe. To
bridge the gap between high strain fatigue and the Paris law, Haigh & Skelton (1978) and Skelton (1982) proposed an equivalent strain range:
εeq =εp +qεe, (26)
whereεeq is the equivalent strain,
εp is the plastic strain,
εe is the elastic strain and
q is a parameter describing the part of the cycle that the crack stays open; a value of 0.5 was chosen based on crack closure measurements by electric conduction across the crack faces. With q=0.5 the εeq is equal to arithmetic mean of
total and plastic strain.
High strain fatigue and linear elastic crack growth can then be unified by defining the strain intensity factor in terms of equivalent strain. This parameter is roughly equal to ∆J (Starkey & Skelton, 1982):
(∆εp +qε πe
( )a 1
Ahmad & Yates (1994) also proposed a fatigue crack growth model based on the Tomkins model. In their model, the Tomkins term was combined with a term for long crack growth to obtain a unified model for cracks growing from notches:
da dN C K T C a m p m = − + (+ ) 5 6 1 2 5 6 ∆ ∆ε , (28)
whereT is a threshold value for crack growth and C5, C6, m5 and m6 are material constants.
More recently Skelton et al. (1998) proposed a model for correlating tested low cycle fatigue (LCF) properties to LEFM fatigue crack growth via an energy-based parameter. In this model the crack growth rate is calculated from the energy required to fail the specimen and the hysteresis energy per cycle, i.e.:
da dN w W J I W f c f f = = +
( )1 1 β β β ∆ , (29)
wherewc is the hysteresis energy per cycle,
Wf is the energy required for failure,
β is a material constant,
Iβ is a constant depending on the value of β and f(β) is 1 for plane stress.
Taira et al. (1976) studied isothermal high temperature low cycle fatigue of 0.16% carbon steel and AISI 304 austenitic stainless steel. They proposed the following crack growth law:
da dN C a m = 7 7 ∆ε , (30)
where C7 and m7 are fitting parameters depending on the material and test
Equation 30 was found to hold for both plastic and total strain range. The exponentm7 was seen to be almost constant over a wide temperature
Figure 7. The temperature dependence of exponent α in equation 30 (after Taira et al., 1976).
Nisitani et al. (1992) proposed the following small crack growth model for stress ranges below the yield stress:
da dN C a m = 8 8 ∆σ , (31)
where C8 and m8 are material parameters.
According to Nisitani et al. (1992) the apparent contradiction between equation 31 and the Paris law (equation 14) can be explained by their different range of applicability. With long cracks and small stresses the crack tip cyclic plastic zone size is proportional to ∆Km1 and the Paris law
describes crack growth. With small cracks and large stresses the small scale yielding condition of LEFM is violated. In this regime, the crack tip plastic zone is given by equation 32 and crack growth rate can be predicted with equation 31. D a y m ∝ σσ 8 , (32)
where D is the plastic zone size.
Nisitani et al. (1992) noted that equation 31 is not suitable for comparing different materials due to differences in the values of the parameters C8 and m8. To overcome this, he proposed the following
equation in which the material properties are partly included:
da dN C y a m = 9 9 ∆σ σ , (33)
Kawagoishi et al. (2000) recently studied the range of applicability of this equation with 0.42% carbon steel. It was shown that the lower limit of applicability of equation 31 is around a crack length of 3 times the grain size of the material (d). Below this value, the strong influence of the microstructure prohibits the use of a mechanical parameter. Microstructural influence continues to be significant until about 8d, but below this value the mean crack growth can be estimated with a mechanical parameter. When cracks grow long enough to satisfy the small scale yielding condition of LEFM, the crack growth becomes ∆ K-controlled, and equation 31 is no longer valid. With higher stress amplitudes, equation 31 is applicable to greater crack lengths. Kawagoishi et al. (2000) described these different regimes of crack growth with the following map (Figure 8).
Figure 8. The applicability of the Paris law (equation 14) and equation 31 as a function of crack length and stress amplitude (after Kawagoishi et al., 2000).
It should be noted that equations 30 and 31 are linearly dependent in the linear-elastic region studied by Nisitani et al. (1992) and Kawagoishi et al. (2000). The equations are equal if:
m7=m8 and (34) C C Em 7 8 8 = , (35)
where E is the Young's modulus.
Fatigue properties of austenitic and duplex stainless steels
The fatigue properties of different stainless steels have been studied widely at different temperatures and environments. Both S-N plots and crack
growth data are widely available in various environments. In Figure 9, the S-N plots for AISI 304 and AISI 316NG stainless steels in air and water are presented. In Figure 10 the crack growth rates of various austenitic stainless steels in different environments are presented. From the presented crack growth data, the material constants C1 and m1 of the Paris law
(equation 14) can be extracted. The extracted values are presented in Table 1. Figure 11 shows the crack growth rate for a duplex stainless steel in air.
Figure 9. S-N plots for AISI 304 and AISI 316NG austenitic stainless steels in air and water (after Chopra & Gavenda, 1998).
Table 1. The material constants C1 and m1 of the Paris law from Figures 10 and 11. Material C m AISI 304, 316, 321, 348 at 25°C 4.6x10-9 3.1 AISI 304 at 593°C 4.7x10-8 2.8 AISI 316 at 593°C 7.3x10-7 2.1 AISI 321 at 593°C 1.2x10-7 2.6 AISI 348 at 593°c 1.2x10-8 3.1 20 Cr, 5.5Ni Duplex at RT 4.6x10-11 3.1
Figure 10. Crack growth data for austenitic stainless steels (after Boyer, 1986).
Figure 11. Crack growth data for A790-grade duplex stainless steels fatigued in air at RT (after Rajanna et al., 1997).
Multiaxial loading shortens expected fatigue life as compared to uniaxial loading. The fatigue life in biaxial loading can be reduced by more than a factor of 2 as compared to uniaxial loading (Itoh et al., 1995; 2000). Numerous models have been proposed to predict the effect of various proportional or nonproportional load paths (e.g., Brown & Miller, 1982; You & Lee, 1996; Socie & Marquis, 2000). The proposed multiaxial fatigue models can be broadly classified into the following approaches (Socie & Marquis, 2000): stress-based models, strain-based models, energy-based models, critical plane models and fracture mechanics models. Stress and strain based models aim to extend the use of the known phenomenological Wöhler or Coffin-Manson models by providing an equivalent damage parameter to be used for multiaxial loading. In energy-based models, the fatigue life is related to the plastic strain energy dissipated during loading. In critical plane models, it is noted that fatigue crack growth can occur predominantly along planes of maximum shear or tensile strain and no single damage model can be expected to be successful for both modes (e.g., Socie, 1987; Socie & Bannantine, 1988). The fracture mechanics models aim to extend crack growth models, such as the Paris law (Equation 14), for mixed mode loading.
Marsh (1981) used the following formulas to convert equi-biaxial thermal fatigue loading to equivalent uniaxial loading:
2 , (36)
where subscripts e and p refer to elastic and plastic, and b and u refer to biaxial and uniaxial loading, respectively. These simple formulas assume, that biaxial loading can be correlated with uniaxial loading by subtracting strain caused by the Poisson effect of the transverse loading (νεeu for elastic
and νeffεpu for the plastic case).
Fatigue crack growth tends to accelerate in aggressive environments. Even fatigue tests conducted in air show significantly higher crack growth rates than tests conducted in vacuum (Wadsworth & Hutchings, 1958). In more aggressive environments, time dependent stress corrosion cracking (SCC) accelerates the crack growth rate. According to McEvily & Wei (1971) and Gabetta et al. (1990) the environmental effects on fatigue crack growth can be divided into true corrosion fatigue (TCF) and stress corrosion fatigue (SCF) (Figure 12).
Figure 12. Separation of corrosion fatigue to true corrosion fatigue and stress corrosion fatigue (after McEvily & Wei, 1971; Gabetta et al., 1990).
In true corrosion fatigue, the crack growth rate follows the conventional Paris law (equation 14), and the environment merely has an effect on changing the material constants C1 and m1 to reflect the
accelerated crack growth rate. The fracture surfaces show ductile features, such as ductile striations, similar to the fracture surfaces produced, e.g., in air.
In stress corrosion fatigue, a time-dependent crack growth component accelerates the crack growth. The fracture surfaces typically show brittle striations or intergranular fracture. The effect of test frequency is decisive. The stress corrosion fatigue crack growth can be correlated to the stress corrosion crack growth under similar environmental and loading conditions.
The maximum expected combined crack growth rate can be expressed as a combination of the crack growth rates caused by true corrosion fatigue and stress corrosion (Gabetta et al., 1990):
da dN da dN t da dN TCF SCC = + , (38)
where the true corrosion fatigue crack growth (subscript TCF) follows the Paris law (equation 14), and stress corrosion crack growth (subscript SCC) is almost constant and can be estimated from slow strain rate test (SSRT) results (Gabetta et al., 1990). The stress corrosion component is present only during the time when the applied ∆K is large enough to exceed the limiting KISCC. This time is a function of the test frequency and is represented by the
Two mechanisms have been suggested to account for the environmental effects on fatigue crack growth: slip oxidation/dissolution (Ford, 1993) and hydrogen-induced cracking (Hänninen et al., 1986). In the former mechanism the crack growth rate is related to the oxidation rate at the strained crack tip and periodicity of oxide rupture at the crack tip. In the latter mechanism crack growth is related to localized hydrogen induced cracking resulting from hydrogen generation due to the corrosion reaction. In stainless steels the fact that fatigue life is longer in water containing low dissolved oxygen than in high dissolved oxygen water suggests that the contribution of slip oxidation/dissolution mechanism is limited (Chopra & Muscara, 2000). Studies on crack initiation in water environments reveal that the observed decrease in fatigue life is caused primarily by the effects of environment on the growth of small cracks less than 500 µm deep (Chopra & Muscara, 2000). The environmental effects depend on strain, dissolved oxygen (DO), strain rate and temperature. The main effects and threshold values of the parameters are summarized in Table 2.
Table 2. The effect of various factors on the decrease of the fatigue life of austenitic stainless steels in aqueous environment (Chopra & Muscara, 2000).
Dissolved oxygen (DO)
The environmental effects are more pronounced in low-DO (<0.01 ppm) than in high-DO water. In high-DO water the environmental effects are moderate when coductivity is low and electrochemical potential (ECP) has reached a stable value. In low-DO water conductivity or additions of lithium and boron have no effect on the fatigue life.
Applied strain A minimum threshold strain is required for the
environmental decrease of fatigue life. During each cycle, the environmental effects are limited to the part of the cycle where the applied strain is above this threshold.
Strain rate In high-DO water with low conductivity and stable ECP, fatigue life is insensitive to strain rate. In low-DO water fatigue life decreases logarithmically with decreasing strain rate below about 0.004 s-1.
Temperature High temperature increases the effect of environment. Environmental effects are minimal below 200°C and become significant above 250°C. Fatigue life is insensitive to changes in temperature in the range of 250 – 330°C.
Higuchi & Iida (1991) have suggested that the effect of environment for austenitic stainless steels can be expressed in terms of fatigue life
correction factor Fen, which is defined as the ratio of life in air at room
temperature to that in water at service temperature. For stainless steels, Fen
can be estimated as follows (Chopra & Muscara, 2000):
Fen=e0 935. − ′ ′ ′Tε˙O , (39) whereT'=0 for T<180°C, T'=(T-180)/40 for 180<T<220°C, T'=1 for T>220°C, ˙ ε'=0 for ε˙>0.004 s-1, ˙ ε'=ln(ε˙/0.004) for 0.000004<ε˙<0.004 s-1, ˙ ε'=ln(0.000004/0.004) for ˙ε<0.000004 s-1,
O'=0.260 for DO<0.05 ppm and O'=0 for DO>0.05ppm.
Corrosion fatigue crack growth in austenitic stainless steels in aqueous environments has been studied extensively (e.g., Kawakubo et al., 1980; Endo et al., 1983; Hishida et al., 1986). Kawakubo et al. (1980) measured crack growth rates of AISI 304 type stainless steel in oxygenated water at 290°C in the solution treated and sensitized conditions (Figure 13).
Figure 13. Crack growth rates of AISI 304 stainless steel in oxygenated water at 290°C (sinusoidal wave loading, frequency 10Hz, stress ratio 0.1, O2 concentration 8 ppm, electrical conductivity <10
S/m) (after Kawakubo et al., 1980).
Dynamic strain ageing
In certain ranges of temperatures and strain rates, many solid solutions exhibit serrated yielding behavior (Portevin–Le Chatelier effect). The phenomenon is explained by interaction between moving dislocations and diffusing solute atoms, i.e. dynamic strain ageing (DSA). According to the model proposed by McCormick (1972), the movement of dislocations during plastic deformation is discontinuous. Dislocations are temporarily arrested at obstacles. They break free and advance with high velocity until they are arrested again at the next obstacle. The average dislocation velocity is determined mainly by the average arrest time spent at the obstacles.
If the arrest time of the dislocation at an obstacle is sufficiently long, the dislocation may be locked by solute atoms, and stress increase is needed for the dislocations to be released from the locking atmosphere formed by the solute atoms. The ageing time required to form the locking atmosphere depends on the diffusion rate of the solute atoms. During plastic deformation, the ageing time decreases due to vacancy production. Dislocation multiplication caused by straining increases the waiting time. At some critical strain the waiting time becomes equal to the required ageing time, and serrated yielding begins (McCormick, 1972).
The strength of the material is increased by dynamic strain ageing. The fracture toughness, ductility and low cycle fatigue resistance are reduced (e.g., Srinivasan et al. 1997). For a given alloy, DSA occurs typically for very limited temperature and strain rate regimes. Dynamic strain ageing is observed in different austenitic stainless steels at temperatures 200–600°C (Srinivasan et al., 1997; Nilsson & Thorvaldsson, 1985; Jenkins & Smith, 1969; Zauter et al., 1993). Due to the limited temperature range of occurence, DSA can cause inverse dependence of strength on temperature, i.e. strength increases with increasing temperature.
Dynamic strain ageing is related to interstitial atoms or interstitial atom-vacancy pairs at temperatures below 500°C and to substititional atoms at higher temperatures. It can be associated with pipe diffusion below 600°C and also with bulk diffusion above 800°C (Ilola, 1999).
Cyclic thermal loads cause fatigue damage and crack growth. If the fatigue loading originates from cyclic pure thermal loads, i.e. thermal loads resulting from internal constraints, then loading is termed thermal fatigue loading. If the loads arise due to external constraints or forces, then the term thermomechanical fatigue is used. The loading is said to be in-phase when the highest temperature coincides with the highest stress and
out-of-phase when the highest temperature coincides with lowest stress (Figure 14).
Figure 14. Schematic illustration of in-phase and out-of-phase loading.
Typically cyclic thermal loads arise from rapid heating or cooling of a component surface, e.g., due to turbulent mixing of fluids of different temperatures. It is characteristic to thermal loads that they are highest at the surface and attenuate towards the inside of the component. The loading is strain-controlled. Because the stresses are self-equilibrating, there exists a surface of zero stress in the component at any given time. This causes the characteristic ∆ε distribution, described schematically in Figure 15, to develop.
Figure 15. Typical distribution of ∆εσ as a function of depth (x) caused by thermal fatigue loading. At any given time the strain distribution shows a point of zero strain (the dashed lines). The corresponding
∆εσ distribution over the whole cycle shows a minimum at a certain distance (the solid line).
The strain range at the surface is often high and exceeds the yield strength of the material. Due to the equilibrating nature of the stresses, residual stresses arise as soon as plastic deformation takes place. Typically, the loading is applied to a surface equally in all directions, and the thermal strains are biaxial.
The characteristics of thermal fatigue loading are reflected in the characteristics of thermal fatigue cracking. The high strains at the surface give rise to rapid crack initiation on a multitude of initiation sites. Because of the biaxiality, cracks initiate and grow equally in all directions and soon form a mosaic-like network. The cracks relax the stresses perpendicular to the crack plane in their vicinity. Hence new cracks turn to meet older cracks at 90° angles. A typical thermal fatigue crack pattern is shown in Figure 16.
Figure 16. Typical mosaic-like crack pattern formed by thermal fatigue.
Due to the rapidly decaying ∆ε seen by a small surface crack, crack growth slows down after the initial rapid growth. Cracks typically slow down at some depth close to the minimum in ∆ε. A smaller number of cracks extend over this minimum and continue to grow with an increasing rate.
Thermomechanical fatigue is closely related to thermal fatigue, although the characteristic features of the load pattern are lost in the case of external constraints or loads. More studies are available on thermomechanical fatigue than pure thermal fatigue probably due to easier comparison and integration to mechanical fatigue testing.
Thermal fatigue studies started, as did mechanical fatigue studies, with empirical tests aimed at providing a simulative verification of a design problem at hand (e.g., Coffin et al., 1954; Coffin & Schenectady, 1954; Tidball & Shrut, 1954). These kinds of studies have continued and S-N curves for different materials and environments have been measured (Hirano et al., 1994; Hayashi 1994; 1998a; 1998b; Hayashi et al., 1998).